Recent Advances of Magnetite (Fe 3 O 4 )-Based Magnetic Materials in Catalytic Applications

: Catalysts play a critical role in producing most industrial chemicals and are essential to environmental remediation. Under the demands of sustainable development, environment protection, and cost-related factors, it has been suggested that catalysts are sufﬁciently separable and conveniently recyclable in the catalysis process. Magnetite (Fe 3 O 4 ) nanomaterials provide a possible way to achieve this goal, due to their magnetism, chemical stability, low toxicity, economic viability, etc. Therefore, Fe 3 O 4 -based materials are emerging as an important solid support to load heterogeneous catalysts and immobilize homogeneous catalysts. Moreover, the addition of magnetic character to catalysts will not only make their recovery much easier but also possibly endow catalysts with desirable properties, such as magnetothermal conversion, Lewis acid, mimetic enzyme activity, and Fenton activity. The following review comprises a short survey of the most recent reports in the catalytic applications of Fe 3 O 4 -based magnetic materials. It contains seven sections, an introduction into the theme, applications of Fe 3 O 4 -based magnetic materials in environmental remediation, electrocatalysis, organic synthesis, catalytic synthesis of biodiesel, and cancer treatment, and conclusions about the reported research with perspectives for future developments. Elucidation of the functions and mechanisms of Fe 3 O 4 nanoparticles (NPs) in these applications may beneﬁt the acquisition of robust and affordable protocols, leading to catalysts with good catalytic activity and enhanced recoverability.


Introduction
Catalysts are one of the fundamental pillars of the chemical industry and have been widely applied in chemical synthesis, energy storage and conversion, biomedical applications, and environmental remediation [1][2][3]. Nanomaterials, which have nano-size intriguing physicochemical properties compared with their bulk materials and excellent reactivities and selectivities, are becoming more and more extensively adopted as catalysts [4]. Conversely, NPs tend to aggregate, which can result in a severe reduction in catalytic activity, and the removal of nanoscopic catalysts from reaction media can be challenging [5,6]. Therefore, NPs with a desirable catalytic activity are commonly loaded in/on a solid support-yielding supported nanocatalyst, and the NPs can be separated from the product accompanying the recovery of support if necessary [7,8]. Aside from NPs, catalysts can also come in the form of water-soluble inorganic matters or organic polymers, such as silicate, transition metal complexes, and ionic liquids (ILs) [9][10][11]. It is evident that green chemistry and environmental protection demand the recovery and reuse of catalysts. In addition to the cost-related factors and operation procedures, it has been suggested that catalysts are easily and completely separated from the product and recycled further [12,13]. In heterogeneous catalytic reaction systems, supported nanocatalysts can be separated via centrifugation and sedimentation with special separation equipment, which is timeconsuming and results in poor recovery and decreased reuse ability of the catalysts [14]. In  [40], Copyright 2021 Elsevier; (B) electrocatalysis [41], Copyright 2018 American Chemical Society; (C) organic synthesis [42], Copyright 2020 Cell Press; (D) synthesis of biodiesel [43], Copyright 2021 Elsevier; (E) drug delivery and cancer treatment [23,44], Copyright 2019 MDPI and Copyright 2020 Elsevier.
In these applications, Fe3O4 universally serves as a form of recyclable support due to its magnetic properties [45]. The link between the magnetic character and catalysts makes their retrieval and reuse much easier, as they can be conveniently separated by using an external magnet, washed, dried, and then subjected to the repeated catalytic reaction, making the catalysis process more sustainable [35,46].
Except for solid support, Fe3O4 can also serve as an Fe-dissolution catalyst towards the activation of H2O2 and persulfate to produce radicals ( • OH, • SO4 − ), which are commonly applied in the oxidation of pollutants [47,48]. This offers Fe3O4-based catalyst, in which Fe3O4 takes the dual responsibility of offering recoverable support and acting as an Fe-dissolution catalyst-the advantages of both homogeneous and heterogeneous catalysts. When grafting catalytically active ILs on Fe3O4 NPs, the generated catalyst can also perform the advantages of homogeneous and heterogeneous catalysts [49,50].  [40], Copyright 2021 Elsevier; (B) electrocatalysis [41], Copyright 2018 American Chemical Society; (C) organic synthesis [42], Copyright 2020 Cell Press; (D) synthesis of biodiesel [43], Copyright 2021 Elsevier; (E) drug delivery and cancer treatment [23,44], Copyright 2019 MDPI and Copyright 2020 Elsevier.

1.
Applications in Environmental Remediation.
Applications in Organic Synthesis. 4.
Applications in Catalytic Synthesis of Biodiesel. 5.
Applications in Cancer Treatment.
This review concludes with observations on the issues that may need to be addressed in further researches regarding catalytic applications of Fe 3 O 4 -based magnetic materials. Continued research into the use of Fe 3 O 4 -based magnetic catalysts is important for the future development of novel recoverable and recyclable catalysts.

Applications in Environmental Remediation
Water is an essential resource for the survival and development of human beings [61]. However, many sources of this essential resource have been contaminated with organic and inorganic pollutants [8]. Organic pollutants predominate in water pollutants and are generally harmful to human health, as many of the organic pollutants have been identified as carcinogenic or mutagenic [62]. These worldwide contaminants are extremely toxic, carcinogenic, biorefractory, and bioaccumulative, even at low concentrations [63]. Therefore, developing a highly effective technique for the removal of these contaminants from water sources is an urgent demand.
As pollutants vary significantly in regard to their physiochemical properties, the remediation methods for pollutants can be very different, including catalytic reduction, catalytic oxidation, catalytic ozonation, photo-assisted oxidation, Fenton catalytic degradation, persulfate catalytic degradation, and so on [64]. Most of these remediation processes require nanocatalysts, the complete removal of which from the reaction solution is as important as the removal of pollutants due to the potential toxic effects of nanocatalysts [65]. Therefore, the expression of superparamagnetism in Fe 3 O 4 -based materials in catalysts may promote the environmental remediation in a green way [36]. On the other hand, Fe 3 O 4 can act as a catalyst in some remediations, such as catalytic reduction, catalytic oxidation, and especially advanced catalytic oxidation reactions [66].

Catalytic Reduction of Pollutants
Nitrophenol, which is vastly found in industrial and agricultural wastewaters, is one of the most common organic-based contaminants [67]. As mine groups are less toxic compared to nitro groups, reducing nitro groups to amines can substantially decrease the toxicity of nitrophenol, which is an important intermediate in the synthesis of various drugs and dyes [68]. However, the reduction of nitrophenol to aminophenol by NaBH 4 in aqueous media is extraordinarily slow due to the kinetic barrier, which is derived from the large potential difference between donor and acceptor molecules, decreasing the feasibility of this reaction [69]. Noble metal NPs are usually adopted as catalysts to promote this reduction [70]. Developing none-noble magnetic catalysts for the catalytic reduction of nitrophenol is very attractive, especially when considering cost and recovery.
Yetim et al. fabricated Fe 3 O 4 and Bi 2 S 3 @Fe 3 O 4 magnetic nanocomposites, both of which show good catalytic reduction ability towards p-nitrophenol with rate constants as high as (1.4-3.8) × 10 −3 min −1 , which are slightly lower than catalysts supported noble NPs ( Figure 2) [71]. Ozkan 4 towards the reduction of p-nitrophenol and excellent magnetism ( Figure 2) [72]. Theses researches showed that Fe 3 O 4 can have a potential catalytic effect in the reduction of nitrophenol, while researches that specifically focus on the catalytic activity of Fe 3 O 4 towards nitrophenol are scarce. Other applications of Fe 3 O 4 -based materials in catalytic reduction also deserve to be explored. large potential difference between donor and acceptor molecules, decreasing the feasibility of this reaction [69]. Noble metal NPs are usually adopted as catalysts to promote this reduction [70]. Developing none-noble magnetic catalysts for the catalytic reduction of nitrophenol is very attractive, especially when considering cost and recovery.
Yetim et al. fabricated Fe3O4 and Bi2S3@Fe3O4 magnetic nanocomposites, both of which show good catalytic reduction ability towards p-nitrophenol with rate constants as high as (1.4-3.8) × 10 −3 min −1 , which are slightly lower than catalysts supported noble NPs ( Figure 2) [71]. Ozkan et al. decorated Co3O4, NiO, and ZnO microparticles with Fe3O4 nanoparticles to obtain Co3O4@Fe3O4, NiO@Fe3O4 and ZnO@Fe3O4 with outstanding magnetic recovery ability. In this research, Fe3O4 exhibited comparable catalytic activity to ZnO@Fe3O4 towards the reduction of p-nitrophenol and excellent magnetism ( Figure 2) [72]. Theses researches showed that Fe3O4 can have a potential catalytic effect in the reduction of nitrophenol, while researches that specifically focus on the catalytic activity of Fe3O4 towards nitrophenol are scarce. Other applications of Fe3O4-based materials in catalytic reduction also deserve to be explored.

Catalytic Oxidation of Pollutants
Despite the fact that the direct catalytic oxidation of pollutants by Fe3O4 NPs has not been reported, enhancements in the catalytic activity of oxidation with the assistance of Fe3O4 NPs-magnetic field and by the incorporation of Fe3O4 NPs with rGO in the production of reactive radicals have been reported, as described in the following.
AsH3, which is generally emitted from phosphorus, sulfurization, and nonferrous metal smelting industries, not only has adverse effects on the biogeochemical cycle and thus poses a major risk to human health due to its relative stability in atmosphere, but can also poison the oxo catalyst and selective catalytic reduction catalyst, thus hindering the utilization of carbon monoxide in the exhaust gas [73]. Therefore, the effective removal of AsH3 in emission gas to its exposure limit of 0.016 mg/m 3 is vitally important. Xie et al. impregnated HZSM-5 zeolite in FeCl3 solution and then fabricated Fe species (including Fe3O4) via calcining. When introducing an external magnetic field (0.1 T) in AsH3 catalytic oxidation, the catalytic performance was improved by 52%, and the turnover frequency value increased from 4.65 × 10 −3 min −1 to 5.73 × 10 −3 min −1 . The alliance of the magnetic field and magnetic materials provides new insights into magnetic-field-assisted catalysis [74].
Premalatha and coworkers prepared a BiOI/rGO/Fe3O4 photocatalyst via the coprecipitation method, which can degrade 98.1% Rhodamine B (20 mg/L, 0.8 g/L catalyst dosage) in 3 h under visible-light-responsive irradiation. The characterizations indicated that the incorporation of rGO and Fe3O4 slowed the electron/hole recombination rate and

Catalytic Oxidation of Pollutants
Despite the fact that the direct catalytic oxidation of pollutants by Fe 3 O 4 NPs has not been reported, enhancements in the catalytic activity of oxidation with the assistance of Fe 3 O 4 NPs-magnetic field and by the incorporation of Fe 3 O 4 NPs with rGO in the production of reactive radicals have been reported, as described in the following. AsH 3 , which is generally emitted from phosphorus, sulfurization, and nonferrous metal smelting industries, not only has adverse effects on the biogeochemical cycle and thus poses a major risk to human health due to its relative stability in atmosphere, but can also poison the oxo catalyst and selective catalytic reduction catalyst, thus hindering the utilization of carbon monoxide in the exhaust gas [73]. Therefore, the effective removal of AsH 3 in emission gas to its exposure limit of 0.016 mg/m 3 is vitally important. Xie et al. impregnated HZSM-5 zeolite in FeCl 3 solution and then fabricated Fe species (including Fe 3 O 4 ) via calcining. When introducing an external magnetic field (0.1 T) in AsH 3 catalytic oxidation, the catalytic performance was improved by 52%, and the turnover frequency value increased from 4.65 × 10 −3 min −1 to 5.73 × 10 −3 min −1 . The alliance of the magnetic field and magnetic materials provides new insights into magnetic-field-assisted catalysis [74].
Premalatha and coworkers prepared a BiOI/rGO/Fe 3 O 4 photocatalyst via the coprecipitation method, which can degrade 98.1% Rhodamine B (20 mg/L, 0.8 g/L catalyst dosage) in 3 h under visible-light-responsive irradiation. The characterizations indicated that the incorporation of rGO and Fe 3 O 4 slowed the electron/hole recombination rate and facilitated the generation of reactive species • OH, resulting in an increased photocatalytic activity (Figure 3) [75].

Advanced Catalytic Oxidation Reactions
Among these environmental remediation techniques, advanced oxidation processes (AOPs) have shown great potential in destroying refractory organic pollutants with high reaction rate constants in the range of 10 8 -10 10 m −1 s −1 [76]. AOPs have a notable performance in the non-selective oxidation of organic pollutants by reactive oxygen species (ROS), such as • OH, • SO4 − , • O2 − , 1 O2, and so on [77]. These free radicals, generated from Fenton reaction, photocatalysis, activated persulfate, ozonolysis, and UV/H2O2 photolysis, can oxidize persistent organic pollutants to low-toxic or non-toxic small molecule substances, and ultimately transform the pollutants to CO2 and H2O [78].
Fe3O4-based materials, with environmentally friendly characteristics, not only exhibit good catalytic performance in heterogeneous Fenton-like reactions for degrading pollutants but also possess a superparamagnetic behavior, which is an essential property for the separation and recovery of catalysts [79].

Fenton Catalytic Degradation of Pollutants
The heterogeneous Fenton system has been widely used in water treatment because of its effective degradability in a wide range of pH levels [80]. Nano-sized magnetic bimetal oxides (Fe3O4, Mn3O4) with highly well-ordered inner-connected structures and large surface areas were fabricated, and the obtained catalysts possessed a higher content of surface-bound Fe(II), which greatly promote the generation of • OHads radicals from Fenton reaction. High toxicity As(III) in water can firstly be oxidized into low toxicity As(V) by • OHfree radicals (69.16%) and bulk solution • OHads radicals (30.39%), then the generated As(V) can be adsorbed by catalysts and be separated from water by a magnet [81].
Li. et al. embedded Fe3O4 NPs into chitosan beads with stable porous structures and abundant active sites to form a porous structure catalyst, which achieves 96.0% degradation of tetracycline (TC, 48.09 mg/L) and six cycles of recycling with negligible catalytic activity loss (Figure 4) [82]. Teng. et al. loaded nano-Fe3O4 on the surface of illite clay via the coprecipitation method, and the resulting catalysts had an excellent degradability of

Advanced Catalytic Oxidation Reactions
Among these environmental remediation techniques, advanced oxidation processes (AOPs) have shown great potential in destroying refractory organic pollutants with high reaction rate constants in the range of 10 8 -10 10 m −1 s −1 [76]. AOPs have a notable performance in the non-selective oxidation of organic pollutants by reactive oxygen species (ROS), such as • OH, • SO 4 − , • O 2 − , 1 O 2 , and so on [77]. These free radicals, generated from Fenton reaction, photocatalysis, activated persulfate, ozonolysis, and UV/H 2 O 2 photolysis, can oxidize persistent organic pollutants to low-toxic or non-toxic small molecule substances, and ultimately transform the pollutants to CO 2 and H 2 O [78]. Fe 3 O 4 -based materials, with environmentally friendly characteristics, not only exhibit good catalytic performance in heterogeneous Fenton-like reactions for degrading pollutants but also possess a superparamagnetic behavior, which is an essential property for the separation and recovery of catalysts [79].

Fenton Catalytic Degradation of Pollutants
The heterogeneous Fenton system has been widely used in water treatment because of its effective degradability in a wide range of pH levels [80]. Nano-sized magnetic bimetal oxides (Fe 3 O 4 , Mn 3 O 4 ) with highly well-ordered inner-connected structures and large surface areas were fabricated, and the obtained catalysts possessed a higher content of surface-bound Fe(II), which greatly promote the generation of • OH ads radicals from Fenton reaction. High toxicity As(III) in water can firstly be oxidized into low toxicity As(V) by • OH free radicals (69.16%) and bulk solution • OH ads radicals (30.39%), then the generated As(V) can be adsorbed by catalysts and be separated from water by a magnet [81].  [84]. Zhang. et al. designed an efficient and recyclable heterogeneous Fenton catalyst (Fe 3 O 4 /reduced graphene oxide aerogel) synthesized via a two-step hydrothermal method for the degradation of methylene blue (MB). The results indicated that MB was firstly adsorbed on the catalysts and then efficiently degraded from pH 3 to pH 10, especially showing a complete degradation in alkaline condition within 60 min. The catalyst can be conveniently recovered by a magnet and exhibits stable catalytic reactivity after five degradation cycles [80]. The possible degradation process can be described as follows (Equations (1)-(3)): bisphenol A (BPA) from real wastewater of 25 mg/L in 180 min with adsorption-Fentonlike mechanism ( Figure 5) [83]. Ye et al. converted Fenton sludge into a magnetic sludgebased biochar through a one-step pyrolysis process and employed it as a novel heterogeneous catalyst to activate H2O2 for the oxidative removal of MB, which exhibited superior catalytic properties and degraded 98.56% of the MB (100 mg/L) in 3 min via the synergistic effects of Fe3O4, Fe 0 , and the biochar. The catalytic ability stood at 88.13% after the 4th run [84]. Zhang. et al. designed an efficient and recyclable heterogeneous Fenton catalyst (Fe3O4/reduced graphene oxide aerogel) synthesized via a two-step hydrothermal method for the degradation of methylene blue (MB). The results indicated that MB was firstly adsorbed on the catalysts and then efficiently degraded from pH 3 to pH 10, especially showing a complete degradation in alkaline condition within 60 min. The catalyst can be conveniently recovered by a magnet and exhibits stable catalytic reactivity after five degradation cycles [80]. The possible degradation process can be described as follows (Equations (1)-(3)):   Similarly, Pan et al. adopted polydopamine as a bridge for connecting Fe 3 O 4 and the pullulan matrix, resulting in the formation of hydrogel containing uniformly distributed Fe 3 O 4 NPs, which showed superior TC degradation efficiency (86.32% within 60 min) by Fenton reaction and can be repeatedly used five times without significant activity loss ( Figure 6) [85]. This strategy solves the problems posed by the poor distribution of magnetic nanoparticles in supported materials and enhances the mechanical properties of the catalysts, which previously severely restricted applications of this type of material from lab to industrial scale. Magnetochemistry 2023, 9, x FOR PEER REVIEW 8 of 32 Similarly, Pan et al. adopted polydopamine as a bridge for connecting Fe3O4 and the pullulan matrix, resulting in the formation of hydrogel containing uniformly distributed Fe3O4 NPs, which showed superior TC degradation efficiency (86.32% within 60 min) by Fenton reaction and can be repeatedly used five times without significant activity loss ( Figure 6) [85]. This strategy solves the problems posed by the poor distribution of magnetic nanoparticles in supported materials and enhances the mechanical properties of the catalysts, which previously severely restricted applications of this type of material from lab to industrial scale.   Similarly, Pan et al. adopted polydopamine as a bridge for connecting Fe3O4 pullulan matrix, resulting in the formation of hydrogel containing uniformly dis Fe3O4 NPs, which showed superior TC degradation efficiency (86.32% within 60 Fenton reaction and can be repeatedly used five times without significant activ ( Figure 6) [85]. This strategy solves the problems posed by the poor distribution netic nanoparticles in supported materials and enhances the mechanical propertie catalysts, which previously severely restricted applications of this type of mater lab to industrial scale.  By combining Fe3O4 and Au NPs, activity of the magnetic recoverable catalyst can be further enhanced. Liu et al. used pine needles as biomass precursors to fabricate N,Odoped magnetic porous carbon and then embedded them with Au NPs, forming a dual active component catalyst, which exhibited outstanding catalytic activity and recyclability toward TC degradation in the presence of H2O2, with a degradation efficiency and degradation rate constant of 96% and 0.133 min −1 within the initial 10 min, respectively ( Figure  7) [86].

Photo-Fenton Catalytic Degradation of Pollutants
In Fenton catalytic degradations, the introduction of visible light into reaction systems can also enhance the degradation of pollutants [87]. Magnetic Cu-Fe oxide derived from Cu-Fe Prussian blue analogue can work as a heterogeneous photo-Fenton catalyst to transform active H2O2 into radicals ( • OH and • O 2− ) under visible light (Vis) and oxidize sulfamethazine (SMZ, 500 mg/L), one of the most commonly used antibiotics, to CO2, H2O, and low-toxic and biodegradable intermediates in just 30 min. The catalysts can be recovered by a magnet due to the presence of Fe3O4, and the catalysts are stable and reusable even after a five-cycle test [88].
A novel core-shell structured Fe3O4@GO@MIL-100(Fe) adopts magnetic Fe3O4 (300-350 nm) as its core and GO (4.5 nm) as its shell, which are then covered by excellent photo responsiveness MIL-100(Fe) (MOFs, thickness is 61 nm). When excited by Vis, MIL-100(Fe) can generate photo-generated electrons and holes, the former of which can be efficiently and quickly transferred to Fe3O4 by GO, leading to almost a 100% degradation of 2,4-DCP within 40 min under the reaction conditions of 3 mmol/L H2O2, 50 mg/L 2,4-DCP, pH 5.5 [89]. The catalyst can be easily recovered under an applied magnetic field and is still available after four cycles ( Figure 8).

Photo-Fenton Catalytic Degradation of Pollutants
In Fenton catalytic degradations, the introduction of visible light into reaction systems can also enhance the degradation of pollutants [87]. Magnetic Cu-Fe oxide derived from Cu-Fe Prussian blue analogue can work as a heterogeneous photo-Fenton catalyst to transform active H 2 O 2 into radicals ( • OH and • O 2− ) under visible light (Vis) and oxidize sulfamethazine (SMZ, 500 mg/L), one of the most commonly used antibiotics, to CO 2 , H 2 O, and low-toxic and biodegradable intermediates in just 30 min. The catalysts can be recovered by a magnet due to the presence of Fe 3 O 4 , and the catalysts are stable and reusable even after a five-cycle test [88].
A novel core-shell structured Fe 3 O 4 @GO@MIL-100(Fe) adopts magnetic Fe 3 O 4 (300-350 nm) as its core and GO (4.5 nm) as its shell, which are then covered by excellent photo responsiveness MIL-100(Fe) (MOFs, thickness is 61 nm). When excited by Vis, MIL-100(Fe) can generate photo-generated electrons and holes, the former of which can be efficiently and quickly transferred to Fe 3 O 4 by GO, leading to almost a 100% degradation of 2,4-DCP within 40 min under the reaction conditions of 3 mmol/L H 2 O 2 , 50 mg/L 2,4-DCP, pH 5.5 [89]. The catalyst can be easily recovered under an applied magnetic field and is still available after four cycles ( Figure 8).
Using TiO 2 decorated on a magnetically activated carbon (TiO 2 @Fe 3 O 4 @Carbon) coupled with ultrasound and ultraviolet can degrade 93% of TC antibiotic under 180 min and can operate stably for five consecutive cycles without any chemical/physical modification [90]. Using TiO2 decorated on a magnetically activated carbon (TiO2@Fe3O4@Carbon) coupled with ultrasound and ultraviolet can degrade 93% of TC antibiotic under 180 min and can operate stably for five consecutive cycles without any chemical/physical modification [90].
Different engineering applications require different Fe3O4 NPs configurations. Alvaro et al. synthesized Fe3O4 monocrystalline nanoflowers with different configurations to suit various engineering applications, such as water remediation, hyperthermia therapy, and enzyme-controlled release. In photo-Fenton-like (visible light irradiation) catalytic reactions, MO can be efficiently degraded within 30 min under visible light irradiation using H2O2 (10 mM). The activity of the catalyst remains relatively high (around 75%) after the fifth cycle, and the amount of dissolved iron only represented 0.4% of the total iron content [91].

Catalytic Activation of Persulfate for the Degradation of Pollutants
Aside from Fenton reaction, the sulfate radical-( • SO4 − ) based advanced oxidation process has emerged as a powerful technique for the degradation and mineralization of organic pollutants, due to its relatively low cost, high efficiency, and ability to degrade refractory organics [92]. • SO4 − can be effectively generated via the catalytic activation of peroxodisulfate (PDS) and peroxymonosulfate (PMS) with transition-metal catalysts (such as Fe, Cu, Mn, and Co-based oxides or composites) through electron transfer reaction [93]. However, the utilization of heavy metal-based catalysts has engendered concerns surrounding toxicity, as the release of metal ions during the persulfate (PS) activation process may cause secondary pollution [94]. As Fe is widely distributed on Earth and generally friendly to the environment and human health, the development of highly stable Fe-based catalysts with a low toxicity has attracted wide interest for practical applications of the PS technique [95].
The fabrication of engineered catalysts with a lower cost, higher activity, and better reusability is challenging for persulfate-based advanced oxidation processes in wastewater treatment. Xiao et al. embedded magnetic bimetallic Fe and Ce into a N-enriched porous biochar (Fe-Ce@N-BC) for peroxymonosulfate activation in metronidazole degradation. The highly dispersed Fe-Ce oxide nanocrystals serve as PMS activation centers and PMS can be efficiently activated via the Fe 2+ /Fe 3+ and Ce 3+ /Ce 4+ pathway, leading

Catalytic Activation of Persulfate for the Degradation of Pollutants
Aside from Fenton reaction, the sulfate radical-( • SO 4 − ) based advanced oxidation process has emerged as a powerful technique for the degradation and mineralization of organic pollutants, due to its relatively low cost, high efficiency, and ability to degrade refractory organics [92]. • SO 4 − can be effectively generated via the catalytic activation of peroxodisulfate (PDS) and peroxymonosulfate (PMS) with transition-metal catalysts (such as Fe, Cu, Mn, and Co-based oxides or composites) through electron transfer reaction [93]. However, the utilization of heavy metal-based catalysts has engendered concerns surrounding toxicity, as the release of metal ions during the persulfate (PS) activation process may cause secondary pollution [94]. As Fe is widely distributed on Earth and generally friendly to the environment and human health, the development of highly stable Fe-based catalysts with a low toxicity has attracted wide interest for practical applications of the PS technique [95].
The fabrication of engineered catalysts with a lower cost, higher activity, and better reusability is challenging for persulfate-based advanced oxidation processes in wastewater treatment. Xiao et al. embedded magnetic bimetallic Fe and Ce into a N-enriched porous biochar (Fe-Ce@N-BC) for peroxymonosulfate activation in metronidazole degradation. The highly dispersed Fe-Ce oxide nanocrystals serve as PMS activation centers and PMS can be efficiently activated via the Fe 2+ /Fe 3+ and Ce 3+ /Ce 4+ pathway, leading to the kinetic reaction rate constant of the Fe-Ce@N-BC/PMS system as high as 5.56 × 10 −2 min −1 in metronidazole degradation. The high loading of iron oxide makes the catalyst magnetically recoverable after use and convenient for recycling [94].
Ye et al. proposed the removal of metals from microplastics, which is achieved by decomposing the organic matter layer that covers the surface of microplastics and releases the adsorbed heavy metal. To realize this goal, they prepared a magnetic biochar with the porosity and graphitization of straw and used K 2 FeO 4 for the heterogeneous catalysis of persulfate activation, which can decrease of more than 60% of the attached Pb on the surface of microplastics. The Pb was subsequently adsorbed by the catalysts and separated from the solution using a magnet [96].
Yang et al. synthesized magnetic Fe 3 O 4 -N-doped carbon sphere composite catalysts for the degradation of tetracycline into CO 2 and H 2 O via activated PMS, achieving a high degradation efficiency of 97.1% within 1 h (C 0 = 20 mg/L, catalyst dosage 0.2 g/L, PMS concentration 2.4 mM, native pH, and 25 • C). Degradation performances between the first and fourth cycles were 93.3%, 79.7%, 80.9%, and 80.9%, respectively, indicating its stable catalytic activity during recycling [97].
Huang et al. used abandoned rape straw as a raw material to synthesize the biochar and loaded Fe 3 O 4 on it, forming a magnetic recyclable rape straw biochar catalyst ( Figure 9). As the Fe 3 O 4 in the catalyst greatly promoted the activation of PS, the catalyst exhibited a high catalytic performance over a wide pH range (2.99-11.01) in the degradation of TC by PS. After being separated by an external magnet, the degradation rate of TC still reached 87.05% after eight cycles, indicating the catalyst has good stability, recoverability, and high practical application value [98]. to the kinetic reaction rate constant of the Fe-Ce@N-BC/PMS system as high as 5.56 × 10 −2 min −1 in metronidazole degradation. The high loading of iron oxide makes the catalyst magnetically recoverable after use and convenient for recycling [94]. Ye et al. proposed the removal of metals from microplastics, which is achieved by decomposing the organic matter layer that covers the surface of microplastics and releases the adsorbed heavy metal. To realize this goal, they prepared a magnetic biochar with the porosity and graphitization of straw and used K2FeO4 for the heterogeneous catalysis of persulfate activation, which can decrease of more than 60% of the attached Pb on the surface of microplastics. The Pb was subsequently adsorbed by the catalysts and separated from the solution using a magnet [96].
Huang et al. used abandoned rape straw as a raw material to synthesize the biochar and loaded Fe3O4 on it, forming a magnetic recyclable rape straw biochar catalyst ( Figure  9). As the Fe3O4 in the catalyst greatly promoted the activation of PS, the catalyst exhibited a high catalytic performance over a wide pH range (2.99-11.01) in the degradation of TC by PS. After being separated by an external magnet, the degradation rate of TC still reached 87.05% after eight cycles, indicating the catalyst has good stability, recoverability, and high practical application value [98]. As the most extensively used brominated flame retardant at present, tetrabromobisphenol A (TBBPA) is an endocrine disruptor and environmental hormone with persistence and biological concentration, which has been proved to have potential neurotoxicity, cytotoxicity and immunotoxicity [99]. Its degradation in nature is extraordinary difficult, thus its effective removal has attracted widespread attention. Hou et al. fabricated a CuFeAl-LDO catalyst containing functional metal oxides (CuOx and Fe3O4) via the hightemperature calcination method and used it for the catalytic degradation of TBBPA by PMS. The degradation rate of TBBPA (15 mg/L) by 0.1 g/L catalyst and 0.5 mM PMS reached 99.91% within 60 min at pH 8.5. The catalyst still maintained high stability and reproducibility after five consecutive repeated degradation reactions of TBBPA. These works provide possible ideas for the application of Fe3O4-based catalysts in the catalytic degradation of brominated phenolic organic pollutants in actual water by PS [100]. As the most extensively used brominated flame retardant at present, tetrabromobisphenol A (TBBPA) is an endocrine disruptor and environmental hormone with persistence and biological concentration, which has been proved to have potential neurotoxicity, cytotoxicity and immunotoxicity [99]. Its degradation in nature is extraordinary difficult, thus its effective removal has attracted widespread attention. Hou

As Support of Catalysts for Environmental Remediation
Metal NPs (MNPs), especially Au NPs, Ag NPs, and Pd NPs, have been widely used in environmental remediation due to their high reactivity and selectivity, which is derived from their unique physicochemical properties when compared with bulk materials [5]. Since NPs are in nano scale (10 −9 m), their separation from the reaction solution poses a big problem. To overcome this issue, MNPs are generally loaded onto a solid support, such as metal oxides, carbon materials, and polymers, in case of aggregation induced by the high surface energy of NPs [102]. When these catalysts are required to be recovered from the reaction solution, it usually requires tedious and time-consuming centrifugationredistribution cycles, during which the noble NPs may leak from the support, resulting in poor recovery of the catalysts and a decrease in catalytic reactivity in the next sequence [103].
Fortunately, as an eco-friendly material, Fe 3 O 4 NPs can be conveniently synthesized and doped in/on other supports with high surface areas or unique features, generating catalysts with magnetic recoverability, high efficiency, renewability, reusability, and high thermal stability. This magnetic technology usually appears as a carrier with a magnetic core or coating and has been developed as a significant separation and recovery method, considering the advantages of fast, efficient, and economical operations.
As listed in Table 2, magnetic catalysts are usually synthesized via multiple steps involving pyrolysis, hydrothermal reaction, solvothermal reaction, microemulsion polymerization, template synthesis, reduction, and so on. Applications of these catalysts in pollutant remediation are the reduction of 4-NP and organic dyes (MB, MO, RhB, CR) and oxidation of BPA, Malathion, Ciprofloxacin, and so on. Benefiting from the magnetism of Fe 3 O 4 , the synthesized catalysts can be conveniently, quickly, and intactly recovered by an external magnet, getting rid of the need for a cumbersome separation process, and making the usage of catalysts more eco-friendly. ) core and stable polydopamine (PDA), which showed excellent catalytic activity in the reaction for reducing azo dyes and excellent antibacterial activity. The catalysts maintained more than 90% activity after five repetitive uses [116].
As Fe 3 O 4 does not participate in the catalytic reaction and is usually coated with modification layers for the accommodation of MNPs, the recyclability of the catalysts can be as high as 99% after 15 cycles of reuse ( Figure 10) [112]. For example, Zhang et al. coated Ag NPs on a magnetic core-shell nanocomposite composed of hollow Fe3O4 (h-Fe3O4) core and stable polydopamine (PDA), which showed excellent catalytic activity in the reaction for reducing azo dyes and excellent antibacterial activity. The catalysts maintained more than 90% activity after five repetitive uses [116].
As Fe3O4 does not participate in the catalytic reaction and is usually coated with modification layers for the accommodation of MNPs, the recyclability of the catalysts can be as high as 99% after 15 cycles of reuse ( Figure 10) [112].

Concepts for the Future
As there are various contaminants in actual polluted water, future researches may focus on the synchronous remediation of multiple pollutants via adsorption-recovery, adsorption-enrichment-degradation, or other effective pathways. Additionally, the multiple pollutants involved in remediation mechanisms should be clarified. Moreover, as the recovery of the catalytic activity after repeated use was commonly low in the reported researches, an Fe3O4-based catalyst with higher stability is required.

Applications in Electrocatalysis
Water electrolysis, which is powered by renewable energy sources, is considered as the most promising technique for the establishment of a clean and sustainable H2 source [121]. Many studies have confirmed that a magnetic catalyst has a spin polarization effect, which may promote a superior electrocatalytic activity and selectivity [121,122]. Adopting

Concepts for the Future
As there are various contaminants in actual polluted water, future researches may focus on the synchronous remediation of multiple pollutants via adsorption-recovery, adsorptionenrichment-degradation, or other effective pathways. Additionally, the multiple pollutants involved in remediation mechanisms should be clarified. Moreover, as the recovery of the catalytic activity after repeated use was commonly low in the reported researches, an Fe 3 O 4 -based catalyst with higher stability is required.

Applications in Electrocatalysis
Water electrolysis, which is powered by renewable energy sources, is considered as the most promising technique for the establishment of a clean and sustainable H 2 source [121]. Many studies have confirmed that a magnetic catalyst has a spin polarization effect, which may promote a superior electrocatalytic activity and selectivity [121,122]. Adopting Fe, an earth-abundant element, for the design of magnetic catalysts is not only an economically viable route for H 2 but could also lead to improved efficiency.
In electrochemical water splitting, the application of Fe 3 O 4 NPs coated with chiral molecules on the anode catalyst (which possesses chiral-induced spin selectivity effect, large surface areas, and abundant reactive sites) can suppress the formation of H 2 O 2 and enhance the triplet oxygen evolution [41]. The mechanism showed that Fe 3 O 4 NPs can induce the spin alignment of electrons in the generated hydroxyl radicals, in addition to the chiral-induced spin selectivity effect, both of which are responsible for the large anode currents of about 10 mA/cm 2 . This finding brings a rational design strategy for highly active anode material by Earth-abundant elements. When an anode composed of magnetic materials (NiZnFe 4 O x ) is placed to a moderate magnetic field (≤450 mT), current density increments are above 100% (over 100 mA/cm 2 ) [121]. Similar research results have been reported in oxygen reduction reaction (ORR), which achieved a strongly enhanced ORR process by applying the external magnetic field and using magnetic materials as cathode catalysts [123].
Magnetic electrocatalysts have also been applied in electrochemical sensing. Prepared with magnetic Fe 3 O 4 NPs, cellulose nanocrystal (CNC), and Cu NPs, Fe 3 O 4 @CNC/Cu was used for modifying a graphite screen-printed electrode and then applied in the analysis of venlafaxine concentration [54]. The experiment results proved that the linear dynamic range was 0.05-600.0 µM, and the limit of detection was 0.01 µM, suggesting that the sensor has good performance for the electrochemical detection of venlafaxine. In addition, the magnetic catalyst can be easily recovered from a reaction mixture using an external magnetic field, which shows promise for the development of a selective, easy, and precise electrochemical sensor to identify special chemicals.
Concepts for the Future: Magnetic electrocatalysts have been applied in electrochemical water splitting and electrochemical sensing due to their remarkable properties, while the mechanism of the specific roles of Fe 3 O 4 NPs in the electrocatalysis process is still ambiguous. The stability and reusability of electrodes need to be improved by the regulation of shape, size, and coating of Fe 3 O 4 NPs and the preparation techniques of electrodes.

Catalytic Hydrogenation/Dehydrogenation
The catalytic upgrading of platform compounds deriving from biomass to fuels and high-value chemicals is more and more appealing because biomass is a sustainable and renewable organic carbon resource generally regarded as a promising substitute for unrenewable fossil resources in producing chemicals and fuels [10]. Furfural (FF), generated from acid-catalyzed hydrolysis and the dehydration process of lignocellulose, is an important platform compound due to its highly functionalized molecular structure [120]. FF can be used as feedstock for the synthesis of furfuryl alcohol (FAOL), which has been widely used for the synthesis of fine chemicals including resins, fibers, and so on. Seeing as adopting H 2 as H donor will increase costs, alcohols and formic acid have been proposed as H donors in the catalytic transfer hydrogenation (CTH) method. Prepared via the coprecipitation method, the acid/base bifunctional Al-Zr@Fe 3 O 4 catalysts showed a high FAOL yield (90.5%) in the hydrogenation of FF by CTH [120]. This magnetic catalyst can be easily recovered by an external magnet and reused for at least five consecutive reaction runs without a significant drop in catalytic activity ( Figure 10). Fe 3 O 4 @C synthesized via the solvothermal method with glucose was adopted in the hydrogenation of FF with isopropanol as a H donor, which achieved a 93.6% conversion of FF and 98.9% yielding of FAOL (200 • C, 4 h) [52]. Fe 3 O 4 takes the role as the Lewis acid catalyst and benefits the recovery of the catalyst through magnetism (Figure 11). Another biomass-derived magnetic Fe 3 O 4 @Zr-FDCA with a core-shell structure was applied in the conversion of ethyl levulinate to γ-valerolactone by CTH, with a yield of 94.5% at 180 • C for 5 h, and recovered by a magnet for repeated use [124]. Both of these two catalysts showed no significant activity loss after four or more cycles.

Catalytic Hydrogenation/Dehydrogenation
The catalytic upgrading of platform compounds deriving from biomass to fuels and high-value chemicals is more and more appealing because biomass is a sustainable and renewable organic carbon resource generally regarded as a promising substitute for unrenewable fossil resources in producing chemicals and fuels [10]. Furfural (FF), generated from acid-catalyzed hydrolysis and the dehydration process of lignocellulose, is an important platform compound due to its highly functionalized molecular structure [120]. FF can be used as feedstock for the synthesis of furfuryl alcohol (FAOL), which has been widely used for the synthesis of fine chemicals including resins, fibers, and so on. Seeing as adopting H2 as H donor will increase costs, alcohols and formic acid have been proposed as H donors in the catalytic transfer hydrogenation (CTH) method. Prepared via the coprecipitation method, the acid/base bifunctional Al-Zr@Fe3O4 catalysts showed a high FAOL yield (90.5%) in the hydrogenation of FF by CTH [120]. This magnetic catalyst can be easily recovered by an external magnet and reused for at least five consecutive reaction runs without a significant drop in catalytic activity ( Figure 10).
Fe3O4@C synthesized via the solvothermal method with glucose was adopted in the hydrogenation of FF with isopropanol as a H donor, which achieved a 93.6% conversion of FF and 98.9% yielding of FAOL (200 °C, 4 h) [52]. Fe3O4 takes the role as the Lewis acid catalyst and benefits the recovery of the catalyst through magnetism (Figure 11). Another biomass-derived magnetic Fe3O4@Zr-FDCA with a core-shell structure was applied in the conversion of ethyl levulinate to γ-valerolactone by CTH, with a yield of 94.5% at 180 °C for 5 h, and recovered by a magnet for repeated use [124]. Both of these two catalysts showed no significant activity loss after four or more cycles. Adopted Pd NPs as a catalyst of hydrogenation and carbonized Fe3O4 as support, Pd@Hal@Glu-Fe3O4-C, achieved a high reactivity on the hydrogenation of five nitroarenes in water at low temperature (40 °C) and high recyclability in repeated uses [127]. Adopted Pd NPs as a catalyst of hydrogenation and carbonized Fe 3 O 4 as support, Pd@Hal@Glu-Fe 3 O 4 -C, achieved a high reactivity on the hydrogenation of five nitroarenes in water at low temperature (40 • C) and high recyclability in repeated uses [127].
As H 2 is in high demand in the new energy industry and chemical industry, various techniques for the production of H 2 have been proposed. Among these techniques, catalytic hydrolysis of NaBH 4 for hydrogen production has attracted considerable attention due to its low operating cost [128]. Due to the advantages of high stability, availability, relatively low cost, and easy separation from reaction reactor, adopting a magnetic catalyst for the generation of H 2 from NaBH 4 has attracted a lot of interest. Soltani et al. prepared CoNi@Fe 3 O 4 @C via the co-deposition-precipitation method, which can be easily separated from the solution at the end of the hydrogen generation cycle and repeated use for six cycles [128].

Catalytic Oxidation
The oxidation and epoxidation of olefins has emerged as a class of essential reactions which is capable of producing various important fine chemicals and intermediates, attracting great interest in academic research and industry [21]. In the oxidation of olefins (styrene) to benzoic acid, Fe 3 O 4 was adopted as support for the fabrication of a recyclable oxidation catalyst, which displayed negligible loss in activity and high selectivity within several successive runs [129].
Supported Fe 3 O 4 NPs on multiwalled carbon nanotubes (Fe 3 O 4 @MWCNT) showed an outstanding performance in the catalytic aqua-thermolysis of heavy asphaltic crude oil. The redox cycle of the Fe 3+ /Fe 2+ species within the Fe 3 O 4 NPs significantly enhanced the oxidization of hydrocarbon molecules, which benefits the upgrading of asphaltic crude oil by reducing its viscosity ( Figure 11). This technique is advantageous due to its low cost in catalyst preparation and catalyst recovery operation, providing a potential opportunity for the industrial exploitation of heavy oil [126].
Sulfoxides are essential in the synthesis of natural products and high-value physiologically and pharmacologically active molecules, and they have received special attention regarding organic synthesis. Synthesized by supporting zirconium on Fe 3 O 4 NPs through creatinine post-functionalization modification, Fe 3 O 4 @Creatinine@Zr offered strong Lewis acid sites for the efficient and selective oxidation of methyl phenyl sulfide to methyl phenyl sulfoxide. The catalyst can be simply separated and recovered by using a magnet and can be reused for seven cycles without any significant decrease in the catalysis activity and selectivity [130].

Catalytic Epoxidation
The selective catalytic conversion of carbohydrates to platform compounds is another way to obtain fuels and fine chemicals from biomass. Thus, the development of efficient solid acidic catalysts with stable catalytic performance is enticing. Various magnetic catalysts with Fe 3 O 4 as support have been applied in the epoxidized catalysis of olefins to organic acid [21]. Fe 3 O 4 @C-SO 3 H, prepared by hydrothermal carbonization of glucose, Fe 3 O 4 grafting, and -SO 3 H group functionalization, can serve as an efficient and recyclable carbon-based solid acidic catalyst in the catalytic dehydration of fructose to 5-hydroxymethylfurfural (HMF) and the subsequent etherification of HMF with ethanol for ethoxymethylfurfural (EMF) [131]. Recycling experiments showed that the catalyst could be easily separated by a magnet and repeatedly used four times consecutively without significant activity loss.

C-C Coupling Reactions
C-C coupling reactions, including the Suzuki, Heck, and other reactions, are one of the valuable routes for the synthesis of fine chemicals via the construction of C-C bonds catalyzed by metal catalysts [5]. The previously described Pd@CMC/Fe 3 O 4 was applied in a model cross-coupling reaction, coupling 4-iodoanisole and phenyl boronicsynthesis for biaryls compounds via Suzuki-Miyaura reactions under microwave irradiation. Reusability studies showed that this magnetic catalyst could be reused for nine cycles without significant activity loss [107]. Another research converted Fe 3 O 4 /SiO 2 support anchoring Pd(II) to Pd@Fe 3 O 4 /SiO 2 by NaBH 4 , and the obtained catalyst performed desirable catalytic activity in the Suzuki-Miyaura cross-coupling of 4-iodobenzene and phenylboronic acid for biphenyl derivatives [132]. The nanocatalyst was reused ten times and the coupling reaction yield varied from 98% to 83% (Figure 12). Similarly, a catalyst prepared by supporting PdNi NPs on dendrimer-functionalized GO@Fe 3 O 4 also performed excellent recyclability in the Suzuki-Miyaura coupling reaction ( Figure 12) [133].

Catalytic Etherification
As a renewable carbohydrate, 5-ethoxymethylfurfural (EMF) is not only desirable for transformation into platform compounds, which can subsequently be transformed to fuels and fine chemicals, but also is a potential biofuel alternative due to its high cetane number deriving from the etherification of the alcoholic functionalized HMF [131]. Therefore, the catalytic etherification of HMF to EMF is vitally important for producing renewable biofuels and fuel additives from biomass. The magnetic catalyst can not only benefit for the separation of the catalyst from the reaction solution but also promote the recycling of the catalyst, thus leading to a cost-effective synthesis technique of advanced biofuel by this magnetic recoverable solid acidic catalyst.
As the etherification of HMF to EMF reactions can be effectively performed in the presence of acid catalysts, previous researches have supported/grafted tungstophosphoric acid (PTA) or sulfonic acid (-SO3H) on Fe3O4-based support (Fe3O4@SiO2, Fe3O4@C) to fabricate a magnetic recoverable catalyst, both of which were used four-five times without significant activity loss [131,134].

Catalytic Etherification
As a renewable carbohydrate, 5-ethoxymethylfurfural (EMF) is not only desirable for transformation into platform compounds, which can subsequently be transformed to fuels and fine chemicals, but also is a potential biofuel alternative due to its high cetane number deriving from the etherification of the alcoholic functionalized HMF [131]. Therefore, the catalytic etherification of HMF to EMF is vitally important for producing renewable biofuels and fuel additives from biomass. The magnetic catalyst can not only benefit for the separation of the catalyst from the reaction solution but also promote the recycling of the catalyst, thus leading to a cost-effective synthesis technique of advanced biofuel by this magnetic recoverable solid acidic catalyst.
As the etherification of HMF to EMF reactions can be effectively performed in the presence of acid catalysts, previous researches have supported/grafted tungstophosphoric acid (PTA) or sulfonic acid (-SO 3 H) on Fe 3 O 4 -based support (Fe 3 O 4 @SiO 2 , Fe 3 O 4 @C) to fabricate a magnetic recoverable catalyst, both of which were used four -five times without significant activity loss [131,134].

Other Catalytic Reactions for Organics
A homogeneous catalyst is superior to a heterogeneous catalyst in terms of mass diffusion and transfer but inferior in terms of recovery and reuse of the catalyst [135]. An approach that centers around the immobilization of a homogeneous catalyst on a magnetic hybrid support to convert it to a heterogeneous catalyst will not only retain the homogeneous activity in the catalytic processes but also achieve the advantage of being recyclable as well as the heterogeneous catalyst. In view of this issue, Maleki et al. decorated SO 3 H-dendrimer on Fe 3 O 4 NPs and applied this heterogeneous-homogeneous catalyst in the one-pot synthesis of polyfunctionalized pyrans and polyhydroquinolines (Figure 13), achieving high product yields and reuse for five cycles with no significant activity loss [136].
Magnetochemistry 2023, 9, x FOR PEER REVIEW 18 of 32 approach that centers around the immobilization of a homogeneous catalyst on a magnetic hybrid support to convert it to a heterogeneous catalyst will not only retain the homogeneous activity in the catalytic processes but also achieve the advantage of being recyclable as well as the heterogeneous catalyst. In view of this issue, Maleki et al. decorated SO3H-dendrimer on Fe3O4 NPs and applied this heterogeneous-homogeneous catalyst in the one-pot synthesis of polyfunctionalized pyrans and polyhydroquinolines (Figure 13), achieving high product yields and reuse for five cycles with no significant activity loss [136]. Kore (Figure 13). The catalyst achieved a 100% conversion and 77% product selectivity in alkylation of benzene with benzyl chloride reaction [35]. Adopting Fe3O4 and nitrogen-doped carbon derived from the thermal processing of natural silk cocoons as support and Cu NPs as an active ingredient, Tahmasbi et al. prepared a Cu@Fe3O4@C catalyst for the synthesis of 5-substituted 1H-tetrazole derivatives by [3+2] cycloaddition reaction of aromatic aldehydes, azide ions, and hydroxylamines [138]. The fabricated catalyst shows considerable reactivity in this [3+2] cycloaddition reactions, and can be reused for five sequential runs without notable reduction in activity.
A recyclable catalyst of Fe3O4@acacia-SO3H was synthesized with acacia gum and iron oxide magnetic NPs, and applied to facilitate the synthesis of 9-phenyl hexahydroacridine pharmaceutical derivatives, which afforded ten cycles of repeated use with a slight activity loss of 9% ( Figure 13) [137]. A catalyst composed of C-SO3H@Fe3O4/C, prepared from Fe3O4 NPs, glucose, and hydroxyethyl-sulfonic acid via one-pot hydrothermal precipitation-sulfonation, was adopted to produce a high yield of glucose (62.59%) and a high yield of total reducing sugar (73.01%) from NaOH-freeze-pretreated sugarcane bagasse [139]. The catalyst could be easily separated and recovered by an external magnetic force at a high recovery rate (93.18%) and could be recycled five times with a glucose yield of 54.47%.  (Figure 13). The catalyst achieved a 100% conversion and 77% product selectivity in alkylation of benzene with benzyl chloride reaction [35].

Concepts for the Future
Adopting Fe 3 O 4 and nitrogen-doped carbon derived from the thermal processing of natural silk cocoons as support and Cu NPs as an active ingredient, Tahmasbi et al. prepared a Cu@Fe 3 O 4 @C catalyst for the synthesis of 5-substituted 1H-tetrazole derivatives by [3+2] cycloaddition reaction of aromatic aldehydes, azide ions, and hydroxylamines [138]. The fabricated catalyst shows considerable reactivity in this [3+2] cycloaddition reactions, and can be reused for five sequential runs without notable reduction in activity.
A recyclable catalyst of Fe 3 O 4 @acacia-SO 3 H was synthesized with acacia gum and iron oxide magnetic NPs, and applied to facilitate the synthesis of 9-phenyl hexahydroacridine pharmaceutical derivatives, which afforded ten cycles of repeated use with a slight activity loss of 9% ( Figure 13) [137]. A catalyst composed of C-SO 3 H@Fe 3 O 4 /C, prepared from Fe 3 O 4 NPs, glucose, and hydroxyethyl-sulfonic acid via one-pot hydrothermal precipitation-sulfonation, was adopted to produce a high yield of glucose (62.59%) and a high yield of total reducing sugar (73.01%) from NaOH-freeze-pretreated sugarcane bagasse [139]. The catalyst could be easily separated and recovered by an external magnetic force at a high recovery rate (93.18%) and could be recycled five times with a glucose yield of 54.47%.

Concepts for the Future
The present section addresses the increasing applicability of Fe 3 O 4 -based nanocatalysts in the process of organic synthesis due to its special properties of superparamagnetism, eco-friendly, high reusability, and high stability in catalysis. However, there is still room for the development of highly efficient methodologies that prepare Fe 3 O 4 -based nanocatalysts with superior dispersibility in the organic phase and high activity retention in recycling, exploiting for synthetic chemistry.

Applications in Catalytic Synthesis of Biodiesel
As a renewable energy source, biodiesel has gained increasing attention for its potential to act as a substitute for the currently used fossil energy due to the non-renewable nature and rapid depletion of fossil energy, and its distinct advantages of being non-poisonous, high cetane number, bio-degradability, renewability, and low emissions [140]. The synthesis of biodiesel is normally accomplished by the transesterification of triglycerides (vegetable oils or animal fats) and alcohols (methanol or ethanol) catalyzed by base catalysts. Homogeneous base catalysts, such as sodium or potassium alkoxide, carbonates, or hydroxide are conventionally used as catalysts on account of their high catalytic activity [141]. Nevertheless, the drawbacks of homogeneous alkaline catalysts, such as the fact that they are non-recoverable and the generation of abundant waste water in the neutralizing and separating processes are major disadvantages that impede the industrial application of homogeneous alkali-catalysts. Therefore, several heterogeneous base catalysts have been investigated for the transesterification processes (Table 3). Among these investigations, magnetic heterogeneous base catalysts have received significant interest due to their advantages of being environmentally benign, ease of separation via magnet, and convenient recyclability, which avoids the leaching of catalyst components into the liquid reaction mixture during traditional filtration and centrifugation.
Xie et al. developed a magnetically recyclable solid catalyst by cross-linking sodium silicate on core-shell Fe 3 O 4 /MCM-41 composites, which exhibited a 99.2% conversion of soybean oil in 8 h at methanol-to-oil molar ratio of 25:1, with a catalyst loading of 3 wt.%. The catalyst can be easily recovered and reused five times without apparent mass loss, and maintained more than 80% catalytic activity [142]. Li et al. synthesized CaO@Fe 3 O 4 with MIL-100(Fe) and calcium acetate, which performed good activity and recyclability in the production of biodiesel with palm oil and methanol ( Figure 14) [143]. Similarly, Carrera et al. synthesized CaO@Fe 3 O 4 from the calcination of the precipitation mixture of Na 2 CO 3 , FeSO 4 , FeCl 3 , Ca(NO 3 ) 2 , and pectin. The catalyst exhibited a methyl ester yield of 99.5% at 3 wt.% catalyst, 14:1 of methanol-to-soybean-oil molar ratio, and 7.5 h of reaction time, while the yield decreased from 99.5% to 21.3% after the fourth cycle, which may be attributable to surface saturation of the catalyst [144]. This reveals that the CaO@Fe 3 O 4 -based biodiesel catalysts have excellent recoverability, which may be enhanced via intermitted activation by a re-calcination.
CaO-ZSM-5 zeolite/Fe 3 O 4 synthesized with ZSM-5 zeolite and CaO also performed excellently in the production of biodiesel with the use of cooking oil and methanol. It showed a biodiesel yield of 91% with a low leached Ca 2+ concentration of 3.87 ppm and a remarkable recyclability of up to four consecutive cycles with a yield over 85% due to the protection of CaO by mesoporous ZSM-5 zeolite (Figure 14) [145].
based biodiesel catalysts have excellent recoverability, which may be enhanced via intermitted activation by a re-calcination.
CaO-ZSM-5 zeolite/Fe3O4 synthesized with ZSM-5 zeolite and CaO also performed excellently in the production of biodiesel with the use of cooking oil and methanol. It showed a biodiesel yield of 91% with a low leached Ca 2+ concentration of 3.87 ppm and a remarkable recyclability of up to four consecutive cycles with a yield over 85% due to the protection of CaO by mesoporous ZSM-5 zeolite (Figure 14) [145].  As sulfonic acid-functionalized ionic liquids (ILs) have a high catalytic activity in the production of biodiesel, Xie et al. grafted dual acidic ILs (1-vinyl-3-(3-sulfopropyl) imidazolium hydrogen sulfate) on the SiO 2 @Fe 3 O 4 composite and implemented it into the synthesis of biodiesel by soybean oil and methanol. Benefiting from the synergism of the homogeneous catalyst and magnetic homogeneous support, the catalyst exhibited excellent catalytic activity and recycling use, which can still achieve a yield of 86% of biodiesel after five cycles [146]. Similarly, an enzyme-like phenylalanine bisulfate ionic liquid (PBIL) grafted on Fe 3 O 4 @GO support not only possess eco-friendly properties but also have superior catalytic activity and recyclability in the synthesis of biodiesel by seed oil and methanol [147].
When Fe 3 O 4 is combined with these biodegradable biomaterials, the catalyst will be aligned with and better prepared for use in the green chemical industry.
Concepts for the Future: The Fe 3 O 4 -based catalyst can be easily recovered from the synthesized biodiesel by applying an external magnetic field, while their catalytic reactivity can suffer a significant decrease upon repeated use, according to the reported studies. Future studies may focus on the solid supporting or grafting of active components of Fe 3 O 4 NPs and the magnetic field-assisted reinforcement of catalytic activity.

Applications in Biological Enzyme Catalysis
Due to their unique advantages of having a low toxicity, mild reaction conditions, and high reaction specificity, enzymes have been used in biotechnology, the food processing industry, and pharmaceutical industry [148], while the extensive industrial application of free enzymes is still subject to their inherent defects associated with instability during storage, vulnerability to inactivation, and lack of recyclability [149]. Thus, the immobilization of enzymes on Fe 3 O 4 -based magnetic recoverable support with enhanced activity and stability has attracted widespread attention. The introduction of Fe 3 O 4 -based magnetic materials makes the immobilized enzyme quickly and easily removable from the reaction solution via an external magnet without damaging the catalyst, providing a perfect way to maintain enzyme activity and their rapid and easy separation from products in a continuous catalytic reaction.
In a recent research, Ren et al. prepared magnetic lipase-Cu 3 (PO 4 ) 2 nanoflowers with lipase, CuCl 2 , amino-functional Fe 3 O 4 NPs, and phosphate-buffered solution, which was applied in the solvent-free biosynthesis of benzyl acetate through benzyl alcohol and vinyl acetate. The amino functionalization of Fe 3 O 4 NPs is essential for the grafting of lipase via crosslinking. The catalyst performed better thermal and pH stability compared with free lipase (at 60 • C and pH 10.0). Additionally, the catalyst can be quickly separated from the reaction system under an external magnetic field, and maintained 57.78% of the initial yield after four consecutive cycles of catalysis [150].
Artificial enzyme mimetics have also attract a lot of interest due to their low cost and stable catalytic activity. It has been proven that Fe 3 O 4 NPs are gifted with an intrinsic enzyme mimetic activity similar to that found in natural peroxidases [151]. In an early study, Fe 3 O 4 NPs were adopted in the colorimetric detection of H 2 O 2 by catalyzing the oxidation of a peroxidase substrate 2,2 -azino-bis(3-ethylbenzo-thiazoline-6-sulfonic acid) diammonium salt with H 2 O 2 to an oxidized colored product, and the detection of glucose by the combination of glucose oxidase and Fe 3 O 4 NP [56].
As more mimetic enzyme characters of Fe 3 O 4 are discovered, Fe 3 O 4 -based materials have been tested in more and more catalytic reactions. Fe 3 O 4 @MIL-100(Fe) synthesized in situ by the microwave-assisted method showed satisfactory intrinsic dual enzyme mimetic activities, including peroxidase-like and catalase-like activities, the former of which was adopted in the design of a biosensor for glutathione detection, and the latter of which was adopted in the catalytic decomposition of H 2 O 2 to quickly produce O 2 and H 2 O [152]. The catalytic activity of both peroxidase and catalase was approximately constant during the recyclability, indicating the high stability and excellent reusability of the nanozyme ( Figure 15).
Inspired by the additional functions of nanomaterials that enhance catalytic activity, the combination of the nano-mimetic enzymes, Fe 3 O 4 , Ag, and MnO 2 were fabricated and tested in peroxidase-like, catalase-like, and oxidase-like activities. The study verified that the combination of nano-mimetic enzymes will endow the Fe 3 O 4 -Ag-MnO 2 with all three of the catalytic activities [153].
Regarding the mechanism and origin of NPs bear not only a higher Fe(II)/Fe(III) ratio but also a more reactive Fe(II) species at surface grain boundaries. This kind of research will not only give us better insights into the origin of Fe 3 O 4 NPs of various crystal forms but also will benefit for the future design of Fe 3 O 4 -based nanozymes [154]. situ by the microwave-assisted method showed satisfactory intrinsic dual enzyme mimetic activities, including peroxidase-like and catalase-like activities, the former of which was adopted in the design of a biosensor for glutathione detection, and the latter of which was adopted in the catalytic decomposition of H2O2 to quickly produce O2 and H2O [152]. The catalytic activity of both peroxidase and catalase was approximately constant during the recyclability, indicating the high stability and excellent reusability of the nanozyme ( Figure 15). Inspired by the additional functions of nanomaterials that enhance catalytic activity, the combination of the nano-mimetic enzymes, Fe3O4, Ag, and MnO2 were fabricated and tested in peroxidase-like, catalase-like, and oxidase-like activities. The study verified that

Applications in Cancer Treatment
Possessing a mild acidity, low catalase activity, hypoxia, and high H 2 O 2 concentration (~(50-100) × 10 −6 M), the tumor microenvironment is not only suitable for tumor development, which finally leads to cancer, but also creates a "gate" for efficient and selective tumor treatments, i.e., the in situ apoptosis inhibits the tumor by employing the Fenton reaction or Fenton-like reactions to produce •OH in tumor sites [155,156].
A composite with two self-activating nanocatalysts was assembled, including the inner core peroxidase-mimic Fe 3 O 4 NPs and the outer glucose oxidase-mimic AuNPs situated within large aperture mesoporous silicon, and subsequently functionalized with cell ligand hyaluronic acid, which can specifically target the receptors of special tumor cells. In treatment, AuNPs can effectively catalyze glucose to produce H 2 O 2 , which is then contiguously catalyzed by Fe 3 O 4 NPs and AuNPs to produce •OH in the tumor microenvironment, ultimately leading to apoptosis and the death of 53.21% of cancer cells without toxicity affecting healthy cells. This composite nanozyme treatment strategy adopting, self-activating ROS-mediated cascade reactions, initiates a non-toxic drug and non-invasive nano-catalytic biomedicine [44].
Other cancer treatment strategies are also proposed in succession, based on the selfaugmented synergistic effects, such as magnetothermal conversion and thermally enhanced Fenton reaction. A novel multifunctional nanosphere that adopted a Fenton catalyst Fe 3 O 4 NPs as the core and photothermal therapy polypyrene as the shell was proposed. In this cancer therapeutic strategy, the multifunctional nanospheres could effectively enrich the tumor site under the guidance of the magnet; then, polypyrene strongly absorbs near-infrared light and converts it into heat for tumor photothermal ablation and effectively promotes Fe 2+/3+ release from Fe 3 O 4 NPs to enhance the catalysis conversion of H 2 O 2 into •OH, leading to the apoptosis of the tumor cell ( Figure 16) [156]. In another research, hollow Fe 3 O 4 meso-crystals took on dual role: (1) magnetic hyperthermia, which can produce heat in the tumor tissue via Fe 3 O 4 and an external magnetic field; (2) Fenton catalyst. This research indicated that meso-crystals of Fe 3 O 4 were superior to polycrystals, not only because the former showed excellent magnetothermal conversion efficiency (722 W/g) but also because they exhibited high peroxidase-like activity in the generation of •OH [60]. Zhang et al. developed engineering encapsulin-produced magnetic iron oxide nanocom-posites with genetically engineered encapsulin protein nanocages via a biomineralization procedure. The magnetic hyperthermia therapy, which contains Fe 3 O 4 and FeO, demonstrated a superior magnetic-to-thermal conversion efficiency (2390 W/g) and performed an enhanced catalase-like activity in the presence of an alternative magnetic field, leading to effective tumor suppression [30]. This integration of magnetic-to-thermal conversion and magnetic-enhancing Fenton catalysis presents a potent tool for cancer treatments.

Concepts for the Future
Considerable efforts have been made in Fe3O4-based medicine for cancer treatment, but their long-term toxicity and metabolization in the human body should be seriously and comprehensively studied before these materials can be safely used to increase life expectancy and prolong cancer patient survival. Further studies may focus on the selective and accurate enrichment of Fe3O4-based medicine in cancerous environments and impose its catalytic activity to generate toxic ROS and kill cancer cells while sparing normal cells. This could be achieved by using strategies such as surface functionalization or cancer-recognizing grafting based on related toxicological mechanisms.

Toxicity of Fe3O4-Based Nanocatalysts in Environmental Remediation and Cancer Treatment
The potential toxicity of Fe3O4-based nanocatalysts is highly concerning, especially in the applications of environmental remediation and cancer treatment.

Toxicity of Fe3O4-Based Nanocatalyst in Environmental Remediation
Studies showed that ~10/100 nm-sized bared Fe3O4 NPs and coated Fe3O4 NPs (Lcysteine, 3-(triethoxysilyl) propylsuccinic anhydride, 3-aminopropyl triethoxysilane, graphitic carbon nitride) demonstrated relatively low toxicity, and did not affect the longterm survival and welfare of the animals at concentrations of 0.001-1 mg/mL [157,158]. Fe3O4 NPs at low concentration can even act as nanonutrition for barley growth [159]. Bared and oxidizing Fe3O4 NPs of ~7 nm (96 h, 3300 mg/L) were proven to not be ecotoxic to plants, while the addition of humic acids or oxidization will increase the inhibitory effect on their unicellular ciliates [160]. Halloysite nanotubes supporting Fe3O4 NPs (~10 nm, 48 h, 200 mg/L) showed no acute toxicity on freshwater organisms [161]. In the application of Fe-dissolution catalysts (activation of H2O2 and persulfate), the dissolved iron ions can be toxic to unicellular ciliates (24 h, 1 mg/L) and slightly toxic to white mustard (96 h, 35 mg/L) [160], while another study indicated that water samples remediated by carbon-supported Fe3O4 (96 h, 500 mg/L) via Fenton reaction exhibited safe effects on aquatic organisms (fish and green algae) in acute and chronic toxicity tests [162].
As Fe3O4 is always adopted as a support, the toxicity of the catalyst should also take

Concepts for the Future
Considerable efforts have been made in Fe 3 O 4 -based medicine for cancer treatment, but their long-term toxicity and metabolization in the human body should be seriously and comprehensively studied before these materials can be safely used to increase life expectancy and prolong cancer patient survival. Further studies may focus on the selective and accurate enrichment of Fe 3 O 4 -based medicine in cancerous environments and impose its catalytic activity to generate toxic ROS and kill cancer cells while sparing normal cells. This could be achieved by using strategies such as surface functionalization or cancerrecognizing grafting based on related toxicological mechanisms.

Toxicity of Fe 3 O 4 -Based Nanocatalysts in Environmental Remediation and Cancer Treatment
The potential toxicity of Fe 3 O 4 -based nanocatalysts is highly concerning, especially in the applications of environmental remediation and cancer treatment.

Toxicity of Fe 3 O 4 -Based Nanocatalyst in Environmental Remediation
Studies showed that~10/100 nm-sized bared Fe 3 O 4 NPs and coated Fe 3 O 4 NPs (L-cysteine, 3-(triethoxysilyl) propylsuccinic anhydride, 3-aminopropyl triethoxysilane, graphitic carbon nitride) demonstrated relatively low toxicity, and did not affect the longterm survival and welfare of the animals at concentrations of 0.001-1 mg/mL [157,158]. Fe 3 O 4 NPs at low concentration can even act as nanonutrition for barley growth [159]. Bared and oxidizing Fe 3 O 4 NPs of~7 nm (96 h, 3300 mg/L) were proven to not be ecotoxic to plants, while the addition of humic acids or oxidization will increase the inhibitory effect on their unicellular ciliates [160]. Halloysite nanotubes supporting Fe 3 O 4 NPs (~10 nm, 48 h, 200 mg/L) showed no acute toxicity on freshwater organisms [161]. In the application of Fe-dissolution catalysts (activation of H 2 O 2 and persulfate), the dissolved iron ions can be toxic to unicellular ciliates (24 h, 1 mg/L) and slightly toxic to white mustard (96 h, 35 mg/L) [160], while another study indicated that water samples remediated by carbonsupported Fe 3 O 4 (96 h, 500 mg/L) via Fenton reaction exhibited safe effects on aquatic organisms (fish and green algae) in acute and chronic toxicity tests [162].
As Fe 3 O 4 is always adopted as a support, the toxicity of the catalyst should also take the potential toxicity of the supported NPs into consideration. Most of the engineered NPs have adverse effects on living organisms, and their nanotoxicology is highly dependent on exposure dosage [163,164]. Therefore, despite the toxicity of some nanocatalysts, their risk of causing environmental and biological damage can be significantly reduced by magnetically recovering them from the reaction system.
Nonetheless, as the leakage of supported NPs, Fe 3 O 4 NPs, and iron ions from nanocatalysts is commonly reported on in current application researches, further studies may focus on the following: (i) improving hybridization strategy to prevent leakage; (ii) developing a deeper understanding of the size, coating, shape, structure, and dosage on environmental fate and toxicity of the nanocatalyst, for the development of biocompatible and biodegradable Fe 3 O 4 -based catalysts.

Toxicity of Fe 3 O 4 -Based Nanocatalyst in Cancer Treatment
When applied in cancer treatment, studies have shown that Fe 3 O 4 NPs may cross the blood-brain barrier and pose potential cytotoxicity-and genotoxicity-related risks to healthy human cells, tissues, and organs via the generation of ROS, which may give rise to lipid peroxidation, mitochondrial dysfunction, chromosomal and DNA damage, leading to protein denaturation and altered cell cycle and gene expression [165,166], while the level of toxicity in Fe 3 O 4 NPs depends on their size, shape, surface coating, dosage, exposure time, and type of cells [167,168]. Poly(acrylic acid) coating on Fe 3 O 4 NPs can significantly reduce their innate toxicity of bared Fe 3 O 4 NPs [169]. A study conducted by Wu et al. indicated that Fe 3 O 4 NPs with a size of 8 nm and coated with polymers could inhibit tumor growth efficiently without expressing obvious toxicity [170]. A toxicity determination test for nanocomposites of reduced graphene oxide, Fe 3 O 4 , and poly-(ethylene) glycol by standard assay revealed over 70% cell survival after 48 h, suggesting that the synthesis of nanocomposites is feasible for magnetic hyperthermia [171]. Whilst plenty of toxicity studies have been carried out in the literature, our collective understanding of the exact fate of Fe 3 O 4 -based materials inside the human body in cancer treatment still remains ambiguous [172].
Therefore, it is essential to comprehensively investigate the toxicity of and potential threat to human health Fe 3 O 4 -based materials pose. This would involve investigating their biocompatibility, biodegradation, biodistribution, on-demand targeting release in the human body, and their fate inside human body. Further studies need to be carried out using in vivo and in vitro models, along with a systematic evaluation of the toxicity of Fe 3 O 4 -based materials and their potential threat to human health, while considering their size, morphology, coating, delivery route, and dosing strategy. In addition, measures and strategies to prevent or shield their toxicity for a safer use in cancer treatment are also required.

Conclusions and Perspectives
In this mini-review, the recent advances in the catalytic applications of Fe 3 O 4 -based magnetic materials are surveyed, such as their applications in environmental remediation, electrocatalysis, organic synthesis, catalytic synthesis of biodiesel, and bio-catalysis. The applications of Fe 3 O 4 -based magnetic materials can be summarized as follows: (1) In the application of environmental remediation, Fe 3 O 4 is usually adopted as a magnetically recoverable support and hybridized with other active ingredients, such as noble metal NPs (Au, Ag, Pd, etc.) and photocatalysts, which have been applied in the oxidized degradation of antibiotics and dyes, as well as the reduction of nitro-benzenes and dyes. Additionally, Fe 3 O 4 is adopted as a recyclable catalyst for the activation of H 2 O 2 and persulfate by dissolving out Fe 2+/3+ and the generated • OH, • SO 4 − , which contribute towards the oxidative decomposition of organic pollutants to low-toxic intermediates such as CO 2, and H 2 O. Fe 3 O 4 -modified catalysts can be easily separated from the reaction solution by an external magnet and exhibit stable catalytic activity during repeated use.
(2) Fe 3 O 4 -based electrocatalysts have been applied in effective and selective electrochemical water splitting so that the spin polarization effect of Fe 3 O 4 can suppress the formation of H 2 O 2 and enhance the triplet oxygen evolution. Designing magnetic catalysts is becoming an economically viable route for H 2 with desirable efficiency. In addition, Fe 3 O 4 NPs can be used for the preparation of selective, easily recoverable, and precise electrochemical sensors to identify special chemicals.
(3) Synthetic chemicals, especially those relating to energy and pharmaceuticals, are essential in the modern world. Fe 3 O 4 NPs are widely adopted as a form of magnetic support in the design of catalysts featuring efficient separation and convenient recycling during the processes of reduction, oxidation, C-C coupling, etherification, and so on. Notably, Fe 3 O 4 can effectively catalyze hydrogenation reactions, in which Fe 3 O 4 takes the role of a Lewis acid catalyst.
(4) Fe 3 O 4 is also used as a magnetically separable support for decorating homogeneous catalysts (acidic ILs) and loading alkali-catalysts, typically being applied in the synthesis of biodiesels via transesterification with various triglycerides and alcohols and making the process more sustainable.
(5) These things considered, Fe 3 O 4 NPs have mimetic peroxidase and catalase activities, thus Fe 3 O 4 NPs have been adopted in the fabrication of artificial enzymes for recyclable catalysis. More importantly, Fe 3 O 4 NPs have been widely employed in cancer treatments, in which Fe 3 O 4 can act as a guide for delivering the therapy to tumor sites under a magnetic field and implement the Fenton reaction for the suppression of cancer cells. The Fenton reaction can be considerably enhanced by the heat that is generated from the magnetothermal conversion of Fe 3 O 4 and photothermal conversion of photothermal materials decorated on Fe 3 O 4 . However, these academic researches cannot be transferred to clinical applications until the obstacles related to the expelling of Fe 3 O 4 outside and the elimination of their long-term toxicity are surmounted.
However, there are some research gaps between the reported studies and the current status. These include the following: (1) When adopting Fe 3 O 4 as a magnetically recoverable support, the flawless recovery of catalytic activity (100%) upon repeated use can be hard to achieve, as seen in the reported researches. Therefore, the connection between the active component and magnetic support is a critical factor for the fabrication of efficient and stable catalysts. An appropriate connection will not only create a suitable space for the active component, preventing the leak of the active component and maintaining catalytic activity during repeated use, but will also promote the sufficient exposure of active sites of the catalyst. Therefore, further researches that aim to obtain highly active and highly recyclable magnetic catalysts, may take the connection styles of Fe 3 O 4 and the active component, crystal form of Fe 3 O 4 (polycrystal, monocrystal), and their surface-decoration/coating in to consideration.
(2) Fe 3 O 4 NPs have mimetic peroxidase and catalase activities and can be used as catalysts of Lewis acid and Fenton reaction, while naked Fe 3 O 4 NPs are subject to oxidation and aggregation, especially under high-temperature reaction conditions, and may cause accountable cytotoxicity in vivo use. To alleviate these restrictions, various strategies, such as supporting, surface coating, and decorating, have been developed to maintain the stability of Fe 3 O 4 or make it biocompatible. However, protecting Fe 3 O 4 from oxidation and aggregation via modification without disturbing catalytic activity is difficult.
In closing, the issues which need to be addressed in future research before their widespread application include: